Hubbard model', B. Valenzuela, M.A.H. Vozmediano, cond-mat ...

The magnetism of the t − t ′ **Hubbard** model

B. **Valenzuela**§† 1 , M.A.H. **Vozmediano**† 2 , and F. Guinea§ 3

§Instituto de Ciencia de Materiales, CSIC

Cantoblanco, 28049 Madrid, Spain.

†Departamento de Matemáticas, Universidad Carlos III de Madrid

Avda. de la Universidad 30, 28913 Leganés (Madrid), Spain.

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

Abstract

The magnetic properties of the t −t ′ **Hubbard** model in the two dimensional square

lattice are studied within an unrestricted Hartree Fock approxi**mat**ion in real space.

The interplay between antiferromagnetism, ferromagnetism, phase separation and inhomogeneous

magnetic textures is studied. It is shown that, at sufficiently large values

of t ′ /t, a rich fenomenology is to be expected between the antiferromagnetic phase at

half filling and the ferromagnetic phase at lower fillings.

PACS numbers: 75.10.Jm, 75.10.Lp, 75.30.Ds.

1 e-mail: belen@jambo.icmm.csic.es

2 e-mail: vozmediano@pinar1.csic.es

3 e-mail: paco.guinea@uam.es

1 Introduction

The single band **Hubbard** model is widely accepted as the simplest starting point of a microscopic

description of correlated electron systems [1]. More recently it has been realized

that inclusion of a t ′ coupling [2] can fit the phenomenology of some cuprates. Recent

photoemission experiments seem to provide Fermi surfaces compatible with the dispersion

relation of the model at moderate values of t ′ and densities [3], while it has been argued

that it can fit some features of ruthenium compounds [4] at higher values of t ′ and the

doping.

The study of inhomogeneous charge and spin phases in the **Hubbard** model has been a

subject of interest since the discovery of the high-T c compounds as it was seen that they

have a very inhomogeneous electronic structure at least in the underdoped regime. However

most of the work was done before the importance of t ′ was realized [5, 6, 7, 8]. A sufficiently

large value of the ratio t ′ /t, compatible with the values suggested for the cuprates

(t ′ /t ∼ −0.3), leads to a significant change in the magnetic properties of the model, as a

ferromagnetic phase appears at low doping. This phase has been found by numerical and

analytical methods [9, 10, 11], and it is a very robust feature of the model.

The purpose of this work is to study the influence of t ′ on the magnetism of the **Hubbard**

model at moderate values of U and density. We will make use of an unrestricted

Hartree-Fock approach in real space what allows us to visualize the charge and spin configurations.

We believe that the method is well suited for the present purposes as: i) it gives

a reasonable description of the Nèel state, with a consistent description of the charge gap

and spin waves, when supplemented with the RPA. ii) It becomes exact if the ground state

of the model is a fully polarized ferromagnet, as, in this case, the interaction plays no role.

A fully polarized ground state is, indeed, compatible with the available Montecarlo[9] and

t-**mat**rix calculations[10]. iii) It is a variational technique, and it should give a reasonable

approxi**mat**ion to the ground state energy. This is the only ingredient required in analyzing

the issue of phase separation. iv) It describes the doped antiferromagnet, for t ′ = 0 as

a dilute gas of spin polarons. The properties of such a system are consistent with other

numerical calculations of the same model [12, 13].

On the other hand, the method used here does not allow us to treat possible super**cond**ucting

instabilities of the model, which have been shown to be present, at least in weak

coupling approaches [11]. The study of these phases requires extensions of the present

approach, and will be reported elsewhere.

The main new feature introduced by a finite t ′ , using simple concepts in **cond**ensed

**mat**ter physics, is the destruction the perfect nesting of the Fermi surface at half filling,

and the existence of a se**cond** interesting filling factor, at which the Fermi surface includes

the saddle points in the dispersion relations. At this filling, the density of states at the

Fermi level becomes infinite, and the metallic phase becomes unstable, even for infinitesimal

values of the interaction. For sufficiently large values of t ′ /t, the leading instability at

this filling is towards a ferromagnetic state.

1

In the following section, we present the model and the method. Then, we discuss the

results. As the system shows a rich variety of behaviors, we have classified the different

regimes into an antiferromagnetic region, dominated by short range antiferromagnetic correlations,

a ferromagnetic one, and an intermediate situation, where the method suggest

the existence of phase separation. The last section presents the main conclusions of our

work.

2 The model and the method

The t-t’ **Hubbard** model is defined in the two dimensional squared lattice by the hamiltonian

H = −t

∑

,s

with the dispersion relation

c + i,s c j,s − t ′

∑

,sc + i,s c j,s + U ∑ i

ε(k) = 2t [cos(k x a) + cos(k y a)] + 4t ′ cos(k x a)cos(k y a) .

n i,↑ n i,↓ , (1)

We have adopted the convention widely used to describe the phenomenology of some

hole-doped cuprates [2], t > 0, t ′ < 0 , 2t ′ /t < 1 . With this choice of parameters the

bandwidth is W = 8t and the Van Hove singularity is approached by doping the half-filled

system with holes. Throughout this study we will fix the value of t = 1 so that energies

will be expressed in units of t. Unless otherwise stated, we will work in a 12 × 12 lattice

with periodic boundary **cond**itions. We have choosen the 12 × 12 lattice because it is the

minimal size for which finite size effects are almost irrelevant [6, 15, 16].

The unrestricted Hartree-Fock approxi**mat**ion minimizes the expectation value of the

hamiltonian (1) in the space of Slater determinants. These are ground states of a single

particle many-body system in a potential defined by the electron occupancy of each site.

This potential is determined selfconsistently

H = − ∑ t ij c † i,s c j,s − ∑ U

2 ⃗m ic † i,s ⃗σ s,s ′c i,s ′ + ∑

i,j,s

i,s,s ′ i

U

2 q i(n i↑ + n i↓ ) + c.c. ,

(where t i,j denotes next, t, and next-nearest, t’, neighbors), and the self-consistency **cond**itions

are

⃗m i = ∑ s,s ′ < c † i,s ⃗σ s,s ′c i,s ′ > , q i =< n i↑ + n i↓ − 1 > ,

where ⃗σ are the Pauli **mat**rices.

We have established a very restrictive criterium for the convergence of a solution. The

iteration ends when the effective potential of the hamiltonian and the one deduced from

the solution are equal up to E < 10 −7 . When different configurations converge for a given

value of the parameters, their relative stability is found by comparing their total energies.

2

3 The results

The results in this work are summarized in fig.1 which represents the energy of the ground

state configurations versus doping from x = 0 to x = 0.34 (where x is the rate of total

number of electrons over the total number of sites) for the representative values t ′ = 0.3

and U = 8. As, in most cases, a variety of selfconsistent solutions can be found, we have

tried to avoid an inital bias by starting with random spin and charge configurations. Once

the system has evolved to a stable final configuration, this has been used as initial **cond**ition

for the nearby dopings. Hence, most of the configurations discussed in the text are robust

in the sense that they have not been forced by a choice of initial **cond**itions and hence are

stable under small changes of the initial values. Exceptions are the diagonal commensurate

domain walls and the stripes. These configurations were set as initial **cond**itions and

found to be self-consistent. Even if there are many possible solutions, the system cannot

be “forced ” to converge to a given solution by appropiately choosing the inital **cond**itions.

In particular homogeneous solutions, such as a pure AF solution, do not converge near half

filling, as will be discussed later. Fig. 2 and fig. 3 show a comparison of the energies of

different configurations converging in the same range of dopings. Fig. 1 shows only minimal

energy configurations. Once a configuration converges, we have checked its stability under

changes in U and t ′ .

The most remarkable feature of fig. 1 is the smooth transition from insulating antiferromagnetism

to metallic ferromagnetism. The antiferromagnetic region extends in a range

of hole doping from x = 0 to x = 0.125 and the ferromagnetic region from x = 0.125 to

x = 0.34. In the antiferromagnetic region the predominant configurations are fully polarized

antiferromagnetism (AF), polarons (POL), diagonal commensurate domain-walls(dcDW),

and noncollinear solutions (S x ). In the ferromagnetic region the phases are ferromagnetic

domains (fm DOM), ferromagnetic non collinear solutions (fm SDW) and the fully polarized

state or Nagaoka configuration (Ng).

Most of the AF configurations are known as solutions of the **Hubbard** model with t ′ = 0

[5, 6, 7, 8, 17, 18]. We will here comment on the changes induced by t ′ . The FM configurations

are totally new and due to the presence of t ′ , as well as the zone of coexistence of

both magnetic orderings. In addition, we have also analyzed in detail some striped configurations,

due to their possible experimental relevance.

In what follows we analyze the antiferromagnetic and ferromagnetic regions and discuss

the possibility of phase separation.

3.1 The antiferromagnetic region

The study of the motion of a few holes in an antiferromagnetic background has been one

of the main subjects in the literature related to the cuprates as these are doped AF insulators.

The region of the **Hubbard** model at and close to half filling is also the area where

the metal-insulator transition [19] occurs, and where the well-established spin polarons or

spin bags [20] coexist with domain walls and, possibly, striped configurations. The diagonal

hopping t ′ has a strong influence over this region as it destroys the perfect nesting of the

3

**Hubbard** model at half filling and the particle-hole symmetry which leads to AFM order

in weak coupling approaches [14, 21].

The AF region is formed by fully polarized antiferromagnetism, polarons, diagonal

commensurante domain-walls and non collinear solutions. We also have found stripes as

excited states. The configurations and the density of states are shown in fig. 4, fig. 5, fig.

6 and fig.7. We will give a brief discussion of these configurations.

Antiferromagnetism

For the reference values of U = 8 and t ′ = 0.3 fully polarized antiferromagnetism

(AF) is the lowest energy configuration only at half filling. For the range of dopings

0.007 ≤ x ≤ 0.027, (1 ≤ h ≤ 4, where h denotes the number of holes), AF converges but

POL are energetically more favourable. Above four holes a purely AF initial configuration

evolves to polarons.

AF is the minimal energy configuration for lower values of U in a wider range of dopings.

For example for U = 4 and t ′ = 0.3 AF is the lowest energy configuration in the range

0 ≤ x ≤ 0.03. This result is almost insensitive to changes in t ′ .

We can conclude then that in the presence of t ′ , the homogeneous fully polarized antiferromagnetic

configuration (Nèel state) is not the dominant solution near half filling. This

result is to be contrasted with what happens with electron doping where AF dominates a

larger region of the doping space. The reason for this asymmetry will become clear in the

discussion of the polaronic configuration following. For t ′ ≠ 0 inhomogeneous solutions are

clearly energetically more favourable.

Polarons

Magnetic polarons have been discussed at length in the literature [20, 8, 22]. For t ′ = 0

the magnetization points along the same direction everywhere in the cluster and the extra

charge is localized in regions that can be of either cigar or diamond shape. These regions

defined a core where the magnetization is reduced.

In the present case, t ′ ≠ 0, this picture changes substantially. The two **Hubbard** bands

in the Nèel state are no longer equivalent, with bandwidths given, approxi**mat**ely, by

8|t ′ | ± 4t 2 /U. Polarons are found at the edges of the narrower band at all values of t’.

This situation corresponds to hole doping for our choice of sign of t ′ ( t ′ /t < 0). The doping

of the wider electron band leads usually to stable homogeneous metallic AF solutions,

where the extra carriers are delocalized throughout the lattice. We have found polarons

in the electron region only when U is big (U > 6) and t’ small (t ′ < 0.15). On the other

hand, the localization of the polarons induced by hole doping increases with increasing

|t ′ /t|. This reflects the fact that these polarons are derived from a narrower **Hubbard** band.

Qualitatively, this fact can be understood in terms of the asymmetric tendency of the system

towards phase separation when t ′ ≠ 0 [23]. The polarons also can be understood as an

incipient form of phase separation, as the core shows strong ferromagnetic correlations.

4

Polarons converge in a wide region of the phase diagram, coexisting with AF and

dcDW as shown in fig. 2. They have lowest energy in the doping range 0.007 ≤ x ≤ 0.035

(1 ≤ h ≤ 5). They do not converge in the range 0.076 ≤ x ≤ 0.097 (11 ≤ h ≤ 13) where the

noncollinear solution has lower energy. This is also different from the situation with t ′ = 0

where polarons converge and have lower energy in the full range of dopings 2 ≤ h ≤ 30 [8].

The DOS of polarons is shown if fig. 5b for five holes. Fig. 5a shows the reference AF state

at half filling. In the DOS for polarons the localized states appear in the antiferromagnetic

gap. As doping increases, they form a mid gap subband but the shape of antiferromagnetic

spectrum is still clearly seen (see fig. 5c).

Diagonal commensurate domain-walls

The dcDW configuration is formed by polarons arranged in the diagonal direction creating

an almost one dimensional charged wall that forms a ferromagnetic domain (see fig.

4b). We stress “commensurate ” because they do not separate different AF domains as

stripes do. The density of states of these solutions differ from that of usual domain walls

in that the one dimensional band where the holes are located is wider, and the Fermi level

lies inside it. We do not find a size independent one particle gap in these solutions, unlike

for conventional domain walls. Within the numerical precision of our calculations, these

structures are metallic, while antiphase domain walls are insulating.

The dcDW are the predominant configuration in the AF region. They converge in the

range of dopings 0.014 ≤ x ≤ 0.118 (2 ≤ h ≤ 17) and are the minimal energy configuration

in most of the doping range as can be seen in fig. 2. These configurations resemble an

array of the polarons discussed earlier, along the (1,1) direction. Thus, we can say that

individual polarons have a tendency towards aligning themselves along the diagonals. This

may be due to the fact that t ′ favors the hopping along these directions. This tendency can

be also seen in the density of states. We have also checked that a lower value of t ′ ( also

for U = 8) these configurations are less favored. In particular for U = 8, dcDW are not

formed at low t ′ while they do form at t ′ = 0.3. Moreover we have tried vertical domain

walls and they are not formed for U = 8 and t ′ = 0.3 but they do with t ′ lower (t ′ = 0.1).

Summarizing, we have checked that t ′ favours dcDW against POL and disfavours vertical

DW. This behaviour is also found with the striped configurations (see below).

Non collinear solution S x

The structure denoted by S x in the phase diagram consists of a special configuration

with noncollinear spin S z . It appears in the range of dopings 0.076 ≤ x ≤ 0.097,

(11 ≤ h ≤ 13), in competition with dcDW and has lower energy. We have checked that

this structure is never seen in the absence of t ′ and is also found at U = 4 and t ′ = 0.3.

The configuration is shown if fig. 4c. We see that there are polarons but there is a

contribution of the spin x at some random sites. The convergence in this configuration

is very slow. It is interesting to point out that we obtain this configuration when using

5

conventional polarons as the initial **cond**ition.

We do not have a complete understanding of why this configuration is preferred in this

region although, it is interesting to note that it happens for the commensurate value of

twelve holes (in our 12 × 12 lattice) and the two neighboring values h = 11 and h = 13.

Its density of states shown in fig. 5d is very similar to the polaronic DOS.

Stripes

The striped configurations are similar to the domain-walls but the one dimensional arrange

of charge separates antiferromagnetic domains with a phase shift of π. Two typical

striped configurations are shown in fig. 6a and fig. 6b. Recently the stripes have attracted

a lot of interest as the half filled vertical stripes (one hole every se**cond** site) are found in

cuprates while diagonal stripes are found in nickelates [24].

We have obtained stripes as higher energy configurations and we have not found half

filled vertical stripes in agreement with other works using mean field approxi**mat**ions for

U = 8 [5, 6, 7, 8, 17]. It is known that the addition of a long range Coulomb interaction

could stabilize the vertical stripes as ground states for large U [25] and applying a slaveboson

version of the Gutzwiller approach the half filled vertical stripes can be ground states

depending on paramenters [26].

We have studied the filled vertical stripe and the diagonal stripe obtained at values of

the doping commensurate with the lattice. Our main interest is the role played by t ′ in

these configurations. We have seen that t ′ has a strong influence on them: t ′ reduces significantly

the basin of attraction of the vertical stripes, what agrees with recent calculations

in the tt ′ − J model [27], while it favors diagonal stripes. The evolution of the vertical

stripe with t ′ can be seen in fig. 6b and fig. 6c for the values U = 4, t ′ = 0 and t ′ = 0.2 .

These stripes do not converge for higher values of t ′ . We have instead found that diagonal

stripes are favored by t ′ much as the dcDW were.

The density of states of the stripes is very similar to that of polarons. We can conclude

that they are insulating states (see fig. 7) unlike the similar commensurate domain walls

where a more metallic character can be appreciated.

3.2 The ferromagnetic region

The existence of metallic ferromagnetism in the **Hubbard** model remains one of the most

controversial issues in the subject [28]. Large areas of ferromagnetism in the doping parameter

were found in the earliest works on the t − t ′ **Hubbard** model within mean field

approxi**mat**ion [14] and were often assumed to be an artifact of the approxi**mat**ion which

would be destroyed by quantum corrections. There are two main regions where ferromagnetism

is likely to be the dominant configuration. One is the region close to half filling, in

particular at one hole doping where the Nagaoka theorem ensures a fully polarized ferromagnetic

state in a bipartite lattice at U = ∞. The other is the region around the Van Hove

fillings where there is a very flat lower band and where ferromagnetism was found for large

6

values of t ′ close to t ′ = 0.5 with quantum Monte Carlo techniques [9] and in the T-**mat**rix

approxi**mat**ion [10]. FM is also found to be the dominant instability for small U and large

t ′ in analytical calculations based on the renormalization group [11], and at intermediate

values of U with a mixture of analytical and mean field calculations [29]. Finally, there is

a controversy on whether Nagaoka ferromagnetism is stabilized at the bottom of the band

ρ → 0 [30].

Most of the previous calculations relay on the study of the divergences of the magnetic

susceptibility pointing to either a symmetry breaking ground state or to the for**mat**ion

of spin density waves as low energy excitations of the system. In many cases it is not

possible in this type of analyses to discern on the precise nature of the magnetic phases,

and, in particular, whether they correspond to fully polarized states (long range order) or

to inhomogeneous configurations with an average magnetization. A complete study of the

magnetic transitions as a function of the electronic density is also a difficult issue.

We have studied the stability of ferromagnetic configurations in the full range of dopings

discussed previously. Two main issues can be addressed within the method of the present

paper. One is the existence of the fully polarized ferromagnetic state (Nagaoka state), and

its stability not only towards the state with one spin flip, but against any weakly polarized

or paramagnetic configuration. The other is the specific symmetry of the partially polarized

ferromagnetic configurations.

In the region close to half filling, our results indicate that the Nagaoka theorem does

probably hold in the presence of t ′ (which spoils the bipartite character of the lattice) since

the Nagaoka state appears when doping with one hole at such large values of U as to make

the kinetic term quite irrelevant. We found Nagaoka FM at values of U such as U = 128.

No FM configurations are found doping with two holes even at U = 128.

The region of low to intermediate electron density has been analyzed for various values

of U and t ′ . This region includes dopings close to the Van Hove singularity where FM

should be enhanced due to the large degeneracy of states in the lower band. The position

of the Van Hove singularity for a given value of U and t ′ can be read off from the undoped

DOS; it has been determined in [31]. Our results are the following:

Nagaoka FM is not found for t ′ = 0.1 at any filling for U ≤ 8. For t ′ = 0.3, two types

of FM configurations are the most stable in the range of dopings shown in fig. 1. Ferromagnetic

spin density waves (fm SDW) despicted in fig. 8b dominate the phase diagram at

densities close to the AFM transition 0.146 ≤ x ≤ 0.194 (21 ≤ h ≤ 28), and in x ≥ 0.264

(h ≥ 37). In the region in between, ferromagnetic domains (fm DOM) as the one shown in

fig. 8c are the most stable. Both types of configurations show a strong charge segregation

and are clearly metallic. The excitation spectrum of these configurations can be seen in

fig. 9.

Fully polarized FM metallic states (Nagaoka) shown in fig. 8a, are found at all values

of h corresponding to closed shell configurations from a critical value h c (U) depending on

t ′ till the bottom of the band. They are shown as vertical solid lines in fig. 1. They are

7

also metallic with a higher DOS at the Fermi level than the partially polarized configurations.

Larger values of t ′ or U push down the critical h in agreement with previous works

[14, 10]. Some values of h c (U) are, for t ′ = 0.3, h c (6) = 37,h c (8) = 29,h c (10) = 21 . For

t ′ = 0.4,h c (8) = 25 . As mentioned before, no FM is found for t ′ = 0.1.

The former results show a large region of ferromagnetic configurations whose upper

boundary coincides with previous esti**mat**ions [10] but which extends to the botton of the

band. We have found paramagnetic configurations to converge in the bottom of the band

but their energies are higher than the ferromagnetic ones. Comparing our solutions with

the corresponding results obtained with the same method in the case t ′ = 0 [8], we find

that the inclusion of t ′ favors ferromagnetism for intermediate to large dopings.

3.3 Phase separation

Although the issue of phase separation (PS) in the **Hubbard** model is quite old [32], it has

become the object of very active research work [33] following the experimental observation

of charge segregation in some cuprates [34]. Despite the effort, the theoretical situation

is quite controversial, although recent calculations rule out PS in the 2D **Hubbard** model

[35, 16]. It seems to occur above some values of J [36, 37, 38], although other work suggests

that it is likely for all values of J in the t − J model [39]. PS has also been invoked in

connection with the striped phase of the cuprates [40].

The theoretical study of PS is a difficult subject. While it is a clear concept in statistical

mechanics dealing with homogeneous systems in thermodynamical equilibrium, the

characterization of PS in discrete systems is much more involved. It is assumed to occur

in those density regions where the energy as a function of density is not a convex function.

This behavior is difficult to achieve in finite systems where the indication of PS is a line,

E(x), of zero curvature, i.e of infinite compressibility. Even this characterization, which

should be correct if it refers to uniform phases of the system, is proble**mat**ic when many

inhomogeneous phases compete in the same region of parameter space. On the other hand,

simple thermodynamic arguments suggest that it should be a general phenomenon near

magnetic phase transitions [41].

PS is also very hard to observe numerically as demonstrated by the results cited previously.

Exact results as the one obtained in [35] are very restrictive and hence of relative

utility.

Our work supports the evidence for phase separation of the model in several ways. The

first is through the plot of the total energy of the minimal energy configuration as a function

of the doping x shown in fig. 1. There we can see that the dominant feature follows a

straight line. As mentioned before, this characterization has the problem of comparing the

energies of different type of configurations.

The evidence is more clear if we observe the same plot for a given fixed configuration in

the AF region where phase separation occurs (fig. 2). The polaronic configurations in fig.

2 follow a straight line while negative curvature is clearly seen in the plot of the commen-

8

surate domain walls, the more aboundant solution in this region. A Maxwell construction

done to this region of curve interpolates rather well to half filling.

The best evidence is provided by the comparison between the plots corresponding to

the two uniform configurations existing in the system. In the case of the Nèel state (AF

of fig. 2) we can see a straight line in the region of densities where it is a self-consistent

solution. This plot should be compared with the one in fig. 10 corresponding to the uniform

Nagaoka states. In the large region where this homogeneous state is found, the plot

follows very closely a standard quadratic curve.

Finally we have looked at the charge and spin configurations of minimal energy. Apart

from the AFM configuration at half filling and the Nagaoka FM, all inhomogeneous configurations

show the same path: coexisting regions of an accumulation of holes accompanied

by a ferromagnetic order with regions of lower density with an AFM order The charge

segregation is obvious in configurations like the ones shown in fig. 4 and in fig. 8c.

We have found fully polarized solutions in closed shell configurations down to the lowest

electron occupancies allowed in our 12 × 12 cluster (5 electrons). However, we cannot rule

out the existence of paramagnetic solutions at even lower fillings.

With all the previous hints we reach the conclusion that the t−t ′ **Hubbard** model tends

to phase separate into an antiferrromagnetic and a ferromagnetic fully polarized state with

different densities for any doping away to half filling up to the Van Hove filling where FM

sets in. It is interesting to note that this result was predicted in a totally different context

by Markiewicz in ref. [42]. Phase separation has also been predicted in the same range of

dopings in ref. [10] but between a paramagnetic and a ferromagnetic state.

4 Conclusions

In this paper we have analyzed the charge and spin textures of the ground state of the

t − t ′ **Hubbard** model in two dimensions as a function of the parameters U, t ′ and the

electron density x in a range from half filling to intermediate hole doping with the aim

of elucidating the role of t ′ on some controversial issues. These include the existence and

stability of ordered configurations such as domain walls or stripes, and the magnetic behavior

in the region of intermediate to large doping where the lower band becomes very flat.

We have used an unrestricted Hartree Fock approxi**mat**ion in real space as the best

suited method to study the inhomogeneous configurations of the system.

Our results are summarized in the representative phase diagram of fig. 1 obtained for

the standard values of the parameters U = 8, t ′ = 0.3. There we can see that the system undergoes

a transition from generalized antiferromagnetic insulating configurations including

spin polarons and domain walls, to metallic ferromagnetic configurations. For the values

of the parameters cited, the transition occurs at an electron density x = 0.125 (h = 18).

Both types of magnetic configurations converge in the intermediate region indicating that

9

the transition is smooth more like a crossover.

The generalized antiferromagnetic configurations are characterized by a large peak in

the density of states of the lower band and by the presence of an antiferromagnetic gap

with isolated polarons for very small doping that evolves to a mid gap subband for larger

dopings. ferromagnetic configurations have a metallic character with a DOS at the Fermi

level that increases for configurations with increasing total magnetization. Fully polarized

Nagaoka states are found at all closed shell configurations in the ferromagnetic zone of the

phase diagram. They have the highest DOS at the Fermi level.

Apart from the homogeneous Néel and Nagaoka states, all inhomogeneous configurations

show the existence of the two magnetic orders associated to charge segregation. AF

is found in the regions of low charge density and FM clusters are formed in the localized

regions where the extra charge tends to accumulate.

Our main conclusion is that the only stable homogeneous phases of the system consists

of the purely antiferromagnetic Nèel configuration at half filling, and Nagaoka ferromagnetism,

which appears around the Van Hove filling. We find the system is unstable towards

phase separation for all intermediate densities.

We have reached this conclusion trough a careful study of the curves representing the

total energy versus doping of the various configurations. Besides, the approach used allows

us to visualize the inhomogeneous configurations. In all of them we find coexisting regions

of an accumulation of holes accompanied by a ferromagnetic order with regions of lower

density with an antiferromagnetic order.

As the ferromagnetic phase is metallic while the Nèel state is insulating, we expect the

transport properties of the model in the intermediate region to resemble that of a percolating

network, a system which has attracted much attention lately [43, 44].

Finally, our study does not exclude the existence of other non magnetic instabilities,

most notably d-wave super**cond**uctivity. This can be, however, a low energy phenomenon,

so that the main magnetic properties at intermediate energies or temperatures are well

described by the study presented here.

We thank R. Markiewicz for a critical reading of the manuscript with very useful comments.

Conversations held with R. Hlubina, E. Louis, and M. P. López Sancho are also

gratefully acknowledged. This work has been supported by the CICYT, Spain, through

grant PB96-0875 and by CAM, Madrid, Spain.

10

References

[1] P.W. Anderson, Science 235, 1196 (1987).

[2] P. Bénard, L. Chen and A. M. Tremblay, Phys. Rev. B. 47, 15 217 (1993); Q. Si, T.

Zha, K. Levin and J. P. Lu, ibid. 47, 9055 (1993).

[3] A. Nazarenko et al., Phys. Rev. B 51, 8676 (1995).

[4] Y. Maeno et al., Nature 372, 532 (1994).

[5] W. P. Su, Phys. Rev. B 37, 9904 (1988).

[6] D. Poilblanc and T.M. Rice, Phys. Rev. B 39, 9749 (1989).

[7] M. Inui and P.B. Littlewood, Phys. Rev. B 44, 4415 (1991).

[8] J. A. Vergés, E. Louis, P. S. Lombdahl. F. Guinea, and A. R. Bishop, Phys. Rev. B

43, 6099 (1991).

[9] R. Hlubina, S. Sorella, and F. Guinea, Phys. Rev. Lett. 78, 1343 (1997).

[10] R. Hlubina, Phys. Rev. B 59, 9600 (1999).

[11] J. V. Alvarez, J. González, F. Guinea, and M. A. H. **Vozmediano**, J. Phys. Soc. Japn.

67, 1868 (1998).

[12] E. Louis, F. Guinea, M. P. López-Sancho and J. A. Vergés, Europhys. Lett. 44, 229

(1998).

[13] E. Louis, F. Guinea, M. P. López-Sancho and J. A. Vergés, Phys. Rev. B, 59, 14005

(1999).

[14] H. Q. Lin and J. E. Hirsch, Phys. Rev. B 35, 3359 (1987).

[15] M. P. López Sancho, J. Rubio, M. C. Refolio, and J. M. López Sancho, Phys. Rev. B

46, 11110 (1992).

[16] A. C. Cosentini, M. Capone, L. Guidoni, and G. B. Bachelet, Phys. Rev. B 58, R14685

(1998).

[17] J. Zaanen and O. Gunnarson, Phys. Rev. B 40, 7391 (1989).

[18] H. J. Schulz, Phys. Rev. Lett. 64, 1445 (1990).

[19] M. Imada, A. Fujimori and Y. Tokura, Rev. Mod. Phys. 70, 1039 (1998).

[20] J. R. Schrieffer, X. -G. Wen, and S. -C. Zhang, Phys. Rev. Lett. 60, 943 (1988).

[21] W. Hofstetter and D. Vollhardt, Ann. Physik 7, 48 (1998).

[22] G. Seibold, E. Sigmund, and V. Hizhnyakov, Phys. Rev. B 57, 6937 (1998).

11

[23] F. Guinea, E. Louis, M. P. López-Sancho and J. A. Vergés, Universality Class of

the Antiferromagnetic Transition in the Two Dimensional **Hubbard** Model, preprint

(**cond**-**mat**/9901164).

[24] J. M. Tranquada, B. J. Sternlieb, J. D. Axe, Y. Nakamura and S. Uchida, Nature

375, 561 (1995); J. M. Tranquada, J. D. Axe, N. Ichikawa, A. R. Moodenbaugh, Y.

Nakamura and S. Uchida, Phys. Rev. Lett. 78, 338 (1997).

[25] J. Zaanen and M. Oleś, Ann. Physik 5, 224 (1996).

[26] G. Seibold, C. Castellani, C. Di Castro and M. Grilli, Phys. Rev. B 58, 13506 (1998).

[27] S. R. White, and D. J. Scalapino **cond**-**mat**/9812187.

[28] For a recent review with a complete list of references see: D. Volhardt, N. Blümer, K.

Held, M. Kollar, J. Schlipf, M. Ulmke, and J. Wahle, Z. Phys. B 103, 283 (1997).

[29] M. Murakami and H. Fukuyama, J. Phys. Soc. Japn. 67, 2784 (1998); M. Murakami,

Possible ordered states in the 2D **Hubbard** model, **cond**-**mat**/9904213.

[30] T. Hanish, G. S. Uhrig, and E. Müller-Hartmann, Phys. Rev. B 56, 13 960 (1997).

See also T. Hanish, G. S. Uhrig, and E. Müller-Hartmann, Lattice dependence of

ferromagnetism in the **Hubbard** model, **cond**-**mat**/9707286.

[31] A. Avella, F. Mancini, D. Villani, and H. Matsumoto, Physika C 282-287, 1759

(1997).

[32] P. B. Visscher, Phys. Rev. B 10, 943 (1974).

[33] For an overview of the subject, see K. A. Müller, and G. Benedek, eds., Proceed. of

the conf. Phase separation in cuprate super**cond**uctors, World Scientific (1993).

[34] J. D. Jorgensen at al., Phys. Rev. B 38, 11 337 (1988); D. R. Harshman et al., Phys.

Rev. Lett. 63, 1187 (1989).

[35] G. Su, Phys. Rev. B 54, R8281 (1996).

[36] V. J. Emery, S. A. Kivelson, and H. Q. Lin, Phys. Rev. Lett. 64, 475 (1990).

[37] E. W. Carlson, S. A. Kivelson, Z. Nussinov and V. J. Emery, Phys. Rev. B 57, 14704

(1998).

[38] M. Calandra, F. Becca and S. Sorella, Phys. Rev. Lett. 81, 5185 (1998).

[39] C. S. Hellberg, and E. Manousakis, Phys. Rev. Lett. 78, 4609 (1997).

[40] J. M. Tranquada et al., Phys. Rev. Lett. 78, 338 (1997).

[41] F. Guinea, G. Gómez-Santos and D. Arovas, **cond**-**mat**/9907184 (preprint).

[42] R. S. Markiewicz, J. Phys. Cond. Matt. 2, 665 (1990).

[43] E. Shimshoni and A. Auerbach, Phys. Rev. B 55, 9817 (1997).

[44] E. Shimshoni, A. Auerbach and A. Kapitulnik, Phys. Rev. Lett. 80, 3352 (1999).

12

5 Figure captions

Fig. 1: Complete phase diagram for U = 8, t’= 0.3. Vertical dashed lines separate the

different configurations described in the text. Vertical solids lines correspond to closed

shells fillings were Nagaoka ferromagnetism occurs. The curve is a plot of the total energy

(in units of t) of the lowest energy configuration versus the electron density x.

Fig. 2: Comparison between the energies of the different configurations converging in

the AF region. The configurations are displayed in fig. 4.

Fig. 3: Comparison between the energies of the configurations in the FM region. The

configurations are displayed in fig. 8.

Fig. 4: Examples of the minimal energy configurations discussed in the text for the

reference values U=8, t’=0.3 in the antiferromagnetic region. Fig. 4a shows the polaronic

(POL) configuration obtained when doping with five holes. Fig. 4b shows the diagonal

commensurate domain wall (dcDW) configuration doping with six holes. Fig. 4c shows

non collinear (S x ) configuration obtained when doping with twelve holes.

Fig. 5: Density of states of the various configurations dicussed in the text in the antiferromagnetic

region for the parameter values U = 8, t’ = 0.3. The fermi level is indicated

as a vertical line. Fig. 5a shows the reference Nèel configuration at half filling. The asymmetry

of the band due to t’ is noticeable. The rest of figures show POL with 5 holes (5b),

POL with 14 holes(5c), dcDW with 6 holes (5d), and the S x configuration with 12 holes (5e).

Fig. 6: Striped configurations appearing at values of the doping commensurate with

the lattice. Fig. 6a. shows the diagonal stripe obtained for the parameter values U = 8 and

t ′ = 0.3. Figs. 6b and 6c correspond to a vertical stripe obtained for U = 4 for the values

of t’ t ′ = 0 (6b), and t ′ = 0.2 (6c). We can see that for bigger t’ the vertical stripe is spoiled.

Fig. 7: Density of states of the diagonal stripe configurations. The Fermi level is indicated

as a vertical line.

Fig. 8: Examples of the minimal energy configurations discussed in the text for the

reference values U=8, t’=0.3 in the ferromagnetic region. Fig. 8a shows the fully polarized

Nagaoka state (Ng) with h=49, fig. 8b shows fmSDW obtained for h= 24, and fig. 8c

corresponds to the fm DOM obtained for h=36.

Fig. 9: Density of states of the ferromagnetic configurations in fig, 8. Fig. 9a corresponds

to the Nagaoka configuration, fig. 9b to fmSDW, and fig. 9c shows the DOS of FM

dom. The Fermi level is indicated as a vertical line.

Fig. 10: Plot of the energy versus doping for the fully polarized Nagaoka configurations

in the full range of dopings where they converge. The solid line is a fit to a quadratic curve.

13

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

−450

Total energy versus doping

(U=8, t’=0.3)

Nagaoka state

−500

total enegy

−550

POL dcDW Sx dcDW fmSDW fm dom fmSDW

−600

−650

0 0.05 0.1 0.15 0.2 0.25 0.3 0.35

x

Energies of different configurations in the AF region

(U=8, t’=0.3)

−595

−605

total energy

−615

−625

−635

pol

Sx

AF

dcDW

−645

0 0.02 0.04 0.06 0.08 0.1 0.12

x

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

Energies of different configurations in the AF region

(U=8, t’=0.3)

−595

−605

total energy

−615

−625

−635

pol

Sx

AF

dcDW

−645

0 0.02 0.04 0.06 0.08 0.1 0.12

x

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

60

DOS of AF

(U=8, t’=0.3, 0 holes)

40

DOS

20

0

−10 −5 0 5 10

energy per part. (in units of t)

50

Density of states of polarons

U=8, t’=0.3, h=5

40

DOS

30

20

10

0

−10 −5 0 5 10

energy per part.(in units of t)

50

Density of states of dcDW

U=8, t’=0.3, h=6

40

DOS

30

20

10

0

−10 −5 0 5 10

energy per part.(in units of t)

50

Density of states of Sx

U=8, t’=0.3, h=12

40

DOS

30

20

10

0

−10 −5 0 5 10

energy per part.(in units of t)

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

40

DOS of diagonal stripes

(U=8, t’=0.3, 11 holes, 11x11 lattice)

30

DOS

20

10

0

−10 −5 0 5 10

energy per part. (in units of t)

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

arXiv:**cond**-**mat**/9909224 v1 15 Sep 1999

20

Density of states of Nagaoka FM

U=8, t’=0.3, h=37

15

DOS

10

5

0

−10 −5 0 5 10

energy per part. (in units of t)

20

Density of states of FM SDW

U=8, t’=0.3, h=24

15

DOS

10

5

0

−10 −5 0 5 10

energy per part.(in units of t)

30

Density of states of FM dom.

U=8, t’=0.3, h=36

20

DOS

10

0

−10 −5 0 5 10

energy per part. (in units of t)

0

Ng points

quadratic curve

Total energy vs doping for Ng state

(U=8, t’=0.3)

total energy

−200

−400

−600

0 0.2 0.4 0.6 0.8 1

x

50

DOS of polarons

U=8, t’=0.3, h=14

40

DOS

30

20

10

0

−10 −5 0 5 10

energy per particle (in units of t)